Araldite Adhesive Bonding
Surface Preparation and Pretreatments
Working directions for the surface preparation essential for optimum adhesion between structural materials bonded with Araldite
Araldite adhesives form extremely strong and durable bonds with plastics, metals, glass, rubber and many other materials. Designers in
every sphere of industry increasingly find that bonding with Araldite adhesives provides the answer to production problems posed by new
materials, new uses of existing materials, joining new techniques and manufacturing methods.
57299_PreTreatUS1.indd 1 6/1/07 11:02:55 AM
Araldite resins adhere firmly to most materials. Bonds of great strength are obtained after removal of grease and loose surface
deposits, e.g. rust, from the surfaces to be joined, but when maximum strength is required a more thorough mechanical or a chemical
pretreatment is recommended.
Surface preparationSurfaces are prepared by one of the following pretreatment procedures (listed in order of increasing effectiveness).
1. Degrease only.
2. Degrease, abrade and remove loose particles.
3. Degrease and chemically pretreat
Care must be taken to avoid contaminating the surfaces during or after pretreatment. Wear clean gloves.
Contamination may be caused by finger marking or by cloths which are not perfectly clean or by oil contaminated abrasives or
by sub-standard degreasing or chemical solutions. Contamination may also be caused by other work processes taking place in the
bonding area. Particularly to be excluded are oil vapours from machinery, spraying operations (paint, mould release-agent, etc.) and
processes involving powdered materials.
Whatever the pretreatment procedure used, it is good practice to bond the surfaces as soon as possible after completion
of the pretreatment i.e. when surface properties are at their best.
Note: If the scheduling of bonding operations on multi-part assemblies causes delay between pretreatment and bonding, optimum
surface properties may be preserved by priming the bond surfaces immediately after pretreatment.
Part 1 Degreasing
The removal of all traces of oil and grease from the surfaces to be bonded is essential. Degreasing by one of the four methods given
below should be carried out even when the surfaces to be bonded appear clean.
Degreasing methodsRemove all traces of oil and grease as follows:
(a) Suspend in a common degreasing solvent such as acetone, MEK, Ethanol or Iso-propanol solvent *vapor in a vapor degreasing
unit. The unit may include a compartment to enable initial washing in the liquid solvent.
where a vapor degreasing unit is not available:
(b) Immerse successively in two tanks each containing the same degreasing solvent. The first tank acts as a wash, the second as a
rinse. When the solvent in the wash tank becomes heavily contaminated, the tank is cleaned out and refilled with fresh solvent.
This tank is then used for the rinse, and the former tank for the wash.
57299_PreTreatUS1.indd 2 6/1/07 11:02:55 AM
(c) Brush or wipe the joint surfaces with a clean brush or cloth soaked in a commercial degreasing solvent. (For fine work, washing
down with solvent applied by aerosol spray may be a more suitable alternative; this technique also ensures that the solvent used is
clean.) Allow to stand for a minute or two to permit complete evaporation from the joint surfaces.
A wide range of proprietary solvent degreasing agents with low hazard ratings are now available. These should be used according
to the manufacturers instructions
(d) Detergent degreasing Scrub the joint surfaces in a solution of liquid detergent. Wash with clean hot water and allow to dry
thoroughly preferably in a stream of hot air from, e.g. a domestic forced-air heater.
Note Non-ionic detergents give generally good results.
(e) Alkaline degreasing is an alternative method to the detergent degreasing.
The ingredients may be selected from a wide range of compounds including sodium or potassium hydroxide, carbonates,
phosphates, borates, complexing agents and organic surfactants. They can be used hot or cold with or without applied
current. There should be very thorough washing, and possibly neutralization to remove residual traces of alkaline cleaners. It is
recommended to use proprietary products and follow manufacturers instructions for use.
(f) Ultrasonic degreasing may be employed when appropriate and is generally used for the preparation of small specimens.
Test for a clean bond surfaceThe water-break test is a simple method to determine whether the surface to be bonded is clean. It is best suited to metals. If a few
drops of distilled water applied to the surface, wet the surface and spread or if, on drawing the surface from distilled water, the water
film does not break up into droplets then the surface may be assumed to be free of contamination. Uniform wetting of the surface by
distilled water indicates that it will probably be likewise wetted by adhesive.
It must be borne in mind that certain plastics, even when clean, may not be wetted by distilled water, but will be wetted by adhesive.
Furthermore, satisfactory wetting gives no information as to the potential bond strength. At most it is a necessary but not sufficient
requirement for the achievement of high bond strengths.
Part 2 Abrading
Lightly abraded surfaces give a better key to adhesives than do highly polished surfaces. Abrasion treatment, if carried out, must be
followed by a further treatment to ensure complete removal of loose particles. For example:
(a) Repeat the degreasing operation (degreasing liquids must be clean), or
(b) Lightly brush with a clean soft brush, or-preferably
(c) Blow with a clean dry (filtered) compressed-air blast.
Metal surfacesRemove surface deposits, e.g. tarnish, rust or mill scale, preferably by blasting with sharp grit*. If grit-blasting equipment is not available
or the metal is too thin to withstand blast treatment, then clean the joint surfaces with a wire brush, or with abrasive cloth or water-
proof abrasive paper (alumina or silicon carbide abrasive, from 46 to 120 mesh). Wetting the wire brush or the abrasive cloth or
paper assists removal of contaminants and reduces dust.
Dry, if necessary, and remove all loose particles.
57299_PreTreatUS1.indd 3 6/1/07 11:02:55 AM
Note Painted surfaces should be stripped of paint; otherwise the strength of the joint may be limited by comparatively low adhesion to metal.
*For most materials the preferred grits are fused alumina and less commonly, silicon carbide (ferrous grits such as chilled iron must be restricted to mild steels and cast irons; their use on other metals may promote corrosion). Fused alumina is the abrasive almost invariably used for aluminum alloys and stainless steels. Silicon carbide is sharper, but it is more expensive and also more friable. Silicon carbide is used on certain special alloys liable to react adversely with any residual fused alumina at temperatures they may encounter in service. The use of silicon carbide can be advantageous when the materials to be abraded are either soft or extremely hard. Choice of grit size depends on various factors: the metal to be grit-blasted, the type of grit-blasting equipment, the pressure and angle of blast impact and the time of treatment. Grits in the range of 46 to 120 mesh are suitable, but the optimum grit size for the work in hand can be determined only by trials. In general for soft materials, the optimum grit size will be towards the fine end of the range.
Plastics and glass surfacesRemove the surface layer of plastics surfaces to ensure elimination of all traces of release agent. As with metals, abrasion by grit-
blasting (see notes on page 3) is in general the best method; the alternative is to use abrasive cloth or paper. After abrasion, remove all
Note Removal of loose particles from plastics surfaces is best carried out by methods (b) or (c) above. Use of degreasing liquids on certain plastics may impair the key produced by the abrasion treatment.
Since plastics are poor heat conductors, care must be taken to keep blasting times as short as possible.
For pretreatment of composite materials cryoblasting may also be used which involves use of solid carbon dioxide pellets as the
Part 3 Pretreatments for particular materials
Most materials, likely to require bonding in industrial practice, are dealt with individually in the following pages for index, see page 15.
Engineers contemplating the bonding of materials not covered by this manual are invited to submit enquiries concerning appropriate
pretreatments to our technical staff.
Special pretreatments for maximum bond performanceThe surface preparation described above, i.e. degreasing alone or degreasing followed by abrasion and removal of loose particles, is
sufficient for most adhesive work.
But to obtain maximum strength, reproducibility and long-term resistance to deterioration, a chemical or electrolytic
pretreatment may be required and examples of these special pretreatments are printed in blue in the following pages.
Metal adherend surfaces are rarely of pure metal, but are a combination of oxides, suphides, chlorides and other atmospheric
contaminants resulting in a surface which is mechanically weak. Acid etching is a w